JOURNAL OF APPLIED PHYSICS

VOLUME 90, NUMBER 7

1 OCTOBER 2001

Dynamic permeability in soft magnetic composite materials A. Chevalier and M. Le Floc’ha) Laboratoire d’Electronique et des Syste`mes de Te´le´communications (L.E.S.T.) UMR CNRS 6616, 6 avenue Le Gorgeu-BP 809-29285 Brest cedex, France

共Received 7 September 2000; accepted for publication 4 June 2001兲 This article reports on an isotropic model of the magnetic susceptibility based on an average field theory and proposes to predict the dynamic behaviors of powder magnetic materials. It was essentially built around a so-called effective demagnetizing factor capable of taking the particle shapes into account. So, for a population of randomly distributed particles of anisotropic shapes like, for instance, needles or flakes, we show that the effective demagnetizing factor of this population of particles can be significantly lowered with regard to the well known value of 1/3 classically used to represent the isotropy state. This phenomenon is interpreted as the natural tendency of particles to form clusters to which a moving demagnetizing factor must be assigned. Taking then the aggregation process of particles into account, the ability of the model to predict the dynamic properties of many composite magnetic materials is successfully demonstrated. Our development is illustrated by experimental results concerning a nickel–zinc ferrimagnetic (Ni0.7Zn0.3Fe2O4) powder. © 2001 American Institute of Physics. 关DOI: 10.1063/1.1389520兴

I. INTRODUCTION

The isotropic character of the mixture is, next, introduced through the assumption of the random distribution of particles in space. The mean internal field 具 H i 典 is derived from the average of the three earlier components

Over the last years the study of composite materials aroused growing interest. We report here on microwave applications of composite materials consisting of soft magnetic particles embedded in insulating binders. Several theories, reviewed by Greffe and Grosse,1 have been proposed to describe the dielectric properties of composite materials. One of the most known among them, the effective medium theory 共EMT兲, has been developed by Bruggeman2 and predicts the average susceptibility of inhomogeneous media. In a previous article3 we showed that, in the simple case of a two-phase mixture where only one of them was magnetic, the EMT leads to a simple and useful scalar expression as follows: 共 1⫺N 兲 2 ⫹ 关 1⫹ 共 N⫺C 兲 i 兴 ⫺C i ⫽0.

具 H i 典 ⫽ 31 共 H i/x ⫹H i/y ⫹H i/z 兲 .

Since the demagnetizing factors satisfy the conditions: N x ⫹N y ⫹N z ⫽1 and N x ⫽N y then, effective data on particle shapes are reduced to the only parameter N z . The internal field 具 H i 典 , then, becomes

具 H i典 ⫽

冋

册

2 H 1 ⫹ . ⫹ 共 i ⫺ 兲共 1⫺N z 兲 /2 ⫹ 共 i ⫺ 兲 N z 3 共3兲

In the meaning of the effective medium theory applied to the isotropic case, we choose to define5,6 the effective shape factor N by taking for 具 H i 典 the same formal expression as that of the H i components

共1兲

The magnetic susceptibility of the mixture depends on the intrinsic susceptibility i of the magnetic substance as well as on the magnetic volume fraction C, and then on the so-called effective shape factor N for the global representation of the microscopic demagnetizing effects. The next part of our study details how the factor N can be connected to the shapes of particles and to their distributions in space.

具 H i典 ⫽

H . 1⫹ 共 i ⫺ / 兲 N

共4兲

The equality between relations 共3兲 and 共4兲, then, allows us to connect N, first to the real parameter of shape N z of the magnetic particles, and second to the volume fraction C. The effective shape factor N is then given by

II. THEORETICAL DEVELOPMENT

In order to simply calculate the effective factor N, we assume that the particles of concern can be replaced by ellipsoids whose the associated triplet of demagnetizing constants (N x , N y , N z ) is fixed by the ratios of the respective lengths of their semi-axes. One can, then, calculate the diagonal tensor4 of the internal field, H i , for such ellipsoid particles of permeability, i , embedded in a homogeneous medium of permeability, 共Fig. 1兲.

N⫽

2⫹3 ␦ N z 共 1⫺N z 兲 , 6⫹ ␦ ⫹3 ␦ N z

共5兲

where ␦ ⫽ i /(1⫹ ) is a so-called factor of contrast, which itself depends on the volume fraction C. The values of N are calculated by solving Eqs. 共1兲 and 共5兲 together. Figure 2 shows that the effective shape factor N depends both on the magnetic load C and on the real shape factor N z of particles. For separated spherical particles N is equal to 1/3 over the whole volume fraction range. On the other hand, in all other cases, i.e., needle- or flake-type par-

a兲

Electronic mail: [email protected]

0021-8979/2001/90(7)/3462/4/$18.00

共2兲

3462

© 2001 American Institute of Physics

Downloaded 19 Oct 2001 to 193.54.253.44. Redistribution subject to AIP license or copyright, see http://ojps.aip.org/japo/japcr.jsp

J. Appl. Phys., Vol. 90, No. 7, 1 October 2001

A. Chevalier and M. Le Floc’h

3463

FIG. 3. Experimental variations of the real part ⬘ of susceptibility of Ni0.7Zn0.3Fe2O4 magnetic composites. FIG. 1. Components of the internal field H i .

ticles, N is smaller than 1/3 so that the shape anisotropy of particles, even for an isotropic mixture, always has the direct consequence to systematically lower the effective shape factor of the mixture. We will now show the ability of the above analytical model 关Eqs. 共1兲 and 共5兲兴 to predict the dynamic properties of soft magnetic powders. In the example chosen, the model is applied to the extraction, from experimental data, of the intrinsic susceptibility i of the magnetic matter. III. EXPERIMENTAL RESULTS

The fine magnetic powders used in our study were synthesized in our laboratory by a wet method7 in order to be sure of the very high chemical purity of the resulting fine powders. Observations by electron microscopy showed that most of the particles were regular and spherical with diameters close to 0.1 m. However, in agreement with the earlier theory, one should keep in mind that clusters can strongly deviate the magnetic properties of the macroscopic body. Composites materials were made by mixing nonmagnetic 共epoxy resin兲 with soft magnetic (Ni0.7Zn0.3Fe2O4 ferrite兲 powders. Then, they were shaped and pressed at room temperature in ring-shaped matrices to avoid the sample de-

FIG. 2. Effective shape factor N as a function of the magnetic load C and of the particle shape factor (N z ). Theoretical values are obtained by solving the couple of Eqs. 共1兲 and 共5兲 for i ⫽20.

magnetizing fields. The magnetic volume fraction ranged within a few percent to about 60%. Thermal densifications were not used in this study. The initial dynamic susceptibility of the composite material 关 ( )⫽ ⬘ ( )⫺ j ⬙ ( ) 兴 was investigated at room temperature in the frequency range 50 MHz–20 GHz by using a Hewlett-Packard APC7 coaxial-line technique and network analyzers. The results are shown in Figs. 3 共real parts兲 and 4 共imaginary parts兲 for different magnetic fractions in the earlier mentioned range. The reduction of the magnetic load lowers the magnitude of the susceptibility. This behavior is general and usually expected. However, as the magnetic resonance frequency 共MRF兲 is spotted by the maximum of the imaginary part of susceptibility, its behavior is clearly different: first, it remains unchanged, then increases continuously below a certain threshold C p close to 30%. We consider this resonance frequency shift as being a direct consequence of the increase of the microscopic demagnetizing fields in the mixture in connection with the modifications of dipolar-type interactions on the one hand, and of the particle arrangements on the other hand. This is quite consistent with other studies which have also clearly highlighted the basic role of the demagnetizing effects8 on the dynamic properties of the magnetic susceptibility in composite materials. As the volume fraction decreases, the local demagnetizing fields add to the total anisotropy field and consequently increase the resonance frequency. In the next

FIG. 4. Experimental variations of the imaginary part ⬙ of susceptibility of Ni0.7Zn0.3Fe2O4 magnetic composites. Full circles 共䊉兲 spot the resonance frequency shift.

Downloaded 19 Oct 2001 to 193.54.253.44. Redistribution subject to AIP license or copyright, see http://ojps.aip.org/japo/japcr.jsp

3464

J. Appl. Phys., Vol. 90, No. 7, 1 October 2001

FIG. 5. Real part of the dynamic intrinsic susceptibility i⬘ obtained with the inversion of experimental data of Fig. 3.

section we will demonstrate that the model proposed in this study takes properly this internal effect into account. IV. COMPARISONS WITH THE MODEL

To process experimental data in order to extract the intrinsic susceptibility of the magnetic matter, we use Eq. 共1兲 in which i is taken as the unknown variable, whereas C and come from measurements. N is then adjusted under the obvious condition that it must remain less than or equal to 1/3. This leads to the noteworthy transformation of Figs. 3 and 4 into the reduced curves of Figs. 5 and 6. One should, indeed, note that, over the whole frequency range and for the different magnetic fractions, there is a unique solution for N; in consequence, the model we use 关see Eq. 共1兲兴 can describe both the decreasing magnitude of the susceptibility and the shift in the MRF observable in composites magnetic materials. Figure 7 shows the experimental values of the earlier solution for N. They correspond to the expected intrinsic susceptibility and are absolutely consistent with the theoretical curves predicted in Fig. 2. They are not only less than 1/3, but they also depend on the volume fraction. V. DISCUSSION

We showed in the previous section that the effective shape factor N depends on both the real particle shape (N z ) and the magnetic fraction C 关Eq. 共5兲兴. Thus, theoretically in the case of spherical particles, the effective shape factor N must be equal to 1/3 and not depend on the magnetic fraction 共see Fig. 2兲. However, experimental values are systematically below 1/3 and magnetic fraction-dependent even in the case of spherical magnetic particles 共Fig. 7兲. This discrepancy, in fact, results from the unavoidable aggregations of

FIG. 6. Imaginary part of the dynamic intrinsic susceptibility i⬙ , obtained with the inversion of experimental data of Fig. 4.

A. Chevalier and M. Le Floc’h

FIG. 7. Experimental and theoretical values of the effective shape factor N obtained to superimpose dynamic spectra of Figs. 5 and 6.

particles during the powder mixing processes, particularly when they are of very small sizes. By way of consequence the clusters are perceived as new particles distorted and bigger than the others. It is then obvious that the shape distribution of such aggregates cannot be evaluated by direct 共microscopy兲 observations, especially because they are sensitive to the changes in the magnetic load. This is, in fact, quite a general problem which largely goes beyond the limits of this study. It is, however, quite possible from simple and practical assumptions to build an intuitive function of distribution of the cluster shapes. First, any aggregation of individual ellipsoidal particles necessarily results in clusters of ellipsoidal shapes with a demagnetizing factor N z 共see Fig. 8兲. Second, the probability P(N z ) to find clusters with a given shape depends on the magnetic fraction as follows: at low concentrations, the particles tend to remain linked in small chainlike aggregates so as they are equivalent to prolate ellipsoids,9 and then the composite becomes equivalent to a mixture of needle-type particles for which N z is by definition less than 1/3. On the contrary, at high concentrations, the clusters grow in any direction and progressively tend to become spherical: by definition, N z is here equal to 1/3. In our study we considered that the probability to develop flake-like aggregates for which N z is by definition higher than 1/3 was unrealistic.

FIG. 8. Identification of aggregates with ellipsoid.

Downloaded 19 Oct 2001 to 193.54.253.44. Redistribution subject to AIP license or copyright, see http://ojps.aip.org/japo/japcr.jsp

J. Appl. Phys., Vol. 90, No. 7, 1 October 2001

A. Chevalier and M. Le Floc’h

3465

When the particle concentration in a given mixture is increasing, aggregates are rapidly formed; their shapes are, then, continuously changing from chains to spheres up to the concentration unity where the medium becomes isotropic. A further work would be in deriving a mathematical function of the distribution P(N z ) to have finally a completely predicting model. This is an interesting challenge because it is known that the dynamic properties of magnetic powder materials are largely influenced by such a term.

VI. CONCLUSION

FIG. 9. Statistical distribution P(N z ) of aggregates shape (N z ) with the volume fraction C.

The earlier assumptions are sufficient to design a convincing profile of the distribution law P(N z ). Indeed, as the magnetic concentration increases, the function P(N z ) must have a maximum whose position is shifted towards the high values of N z up to 1/3 共strictly speaking兲 when the magnetic fraction reaches unity. Simultaneously, the profile of P(N z ) must become narrower and narrower. Figure 9, finally, shows the histogram of P(N z ) which was used to realize the very satisfactory fit of Fig. 7. For an exact computation of the effective shape factor N, Eq. 共3兲 can be now easily expressed as a continuous sum acting on N z as follows:

具 H i典 ⫽

冕 冋 1

0

⫹

2 ⫹ 共 i ⫺ 兲共 1⫺N z 兲 /2

册

H 1 P 共 N z 兲 dN z . ⫹共 i⫺ 兲N z 3

共6兲

An extension of the effective medium theory was proposed to predict the dynamic behaviors of isotropic composite materials. This model is capable of describing experimental results, namely the variation of magnitude of permeability, together with the shift of the resonance frequency. While taking into account the formation of particle aggregates, we derived the intrinsic permeability of magnetic matter independently of the magnetic fraction of the mixture. An immediate and interesting extension of this work would be the determination of an analytical function of the magnetic fraction of the mixture to take the grain structure contribution into account.

1

J. L. Greffe and Grosse, Dielectric Properties of Heterogeneous Materials, P.I.E.R. 6 共Elsevier, New York, 1992兲. 2 D. A. G. Bruggeman, Ann Phys. 共Leipzig兲 24 共1935兲. 3 M. Le Floc’h, J. L. Mattei, P. Laurent, O. Minot, and A. M. Konn, J. Magn. Magn. Mater. 140 共1995兲. 4 J. A. Stratton, Electromagnetic Theory 共McGraw-Hill, New York, 1941兲. 5 M. Le Floc’h, A. Chevalier, and J. L. Mattei, J. Phys. IV 8, 2 共1998兲. 6 A. Chevalier, Ph.D. thesis, Universite´ de Bretagne Occidentale, 1998. 7 T. Takada and M. Kiyama, Proc. Of Intern. Conf., Japan 1970, p. 69. 8 C. Kittel, Phys. Rev. 73, 155 共1948兲. 9 C. G. Granqvist and O. Hunderi, Phys. Rev. B 18, 1554 共1978兲.

Downloaded 19 Oct 2001 to 193.54.253.44. Redistribution subject to AIP license or copyright, see http://ojps.aip.org/japo/japcr.jsp

VOLUME 90, NUMBER 7

1 OCTOBER 2001

Dynamic permeability in soft magnetic composite materials A. Chevalier and M. Le Floc’ha) Laboratoire d’Electronique et des Syste`mes de Te´le´communications (L.E.S.T.) UMR CNRS 6616, 6 avenue Le Gorgeu-BP 809-29285 Brest cedex, France

共Received 7 September 2000; accepted for publication 4 June 2001兲 This article reports on an isotropic model of the magnetic susceptibility based on an average field theory and proposes to predict the dynamic behaviors of powder magnetic materials. It was essentially built around a so-called effective demagnetizing factor capable of taking the particle shapes into account. So, for a population of randomly distributed particles of anisotropic shapes like, for instance, needles or flakes, we show that the effective demagnetizing factor of this population of particles can be significantly lowered with regard to the well known value of 1/3 classically used to represent the isotropy state. This phenomenon is interpreted as the natural tendency of particles to form clusters to which a moving demagnetizing factor must be assigned. Taking then the aggregation process of particles into account, the ability of the model to predict the dynamic properties of many composite magnetic materials is successfully demonstrated. Our development is illustrated by experimental results concerning a nickel–zinc ferrimagnetic (Ni0.7Zn0.3Fe2O4) powder. © 2001 American Institute of Physics. 关DOI: 10.1063/1.1389520兴

I. INTRODUCTION

The isotropic character of the mixture is, next, introduced through the assumption of the random distribution of particles in space. The mean internal field 具 H i 典 is derived from the average of the three earlier components

Over the last years the study of composite materials aroused growing interest. We report here on microwave applications of composite materials consisting of soft magnetic particles embedded in insulating binders. Several theories, reviewed by Greffe and Grosse,1 have been proposed to describe the dielectric properties of composite materials. One of the most known among them, the effective medium theory 共EMT兲, has been developed by Bruggeman2 and predicts the average susceptibility of inhomogeneous media. In a previous article3 we showed that, in the simple case of a two-phase mixture where only one of them was magnetic, the EMT leads to a simple and useful scalar expression as follows: 共 1⫺N 兲 2 ⫹ 关 1⫹ 共 N⫺C 兲 i 兴 ⫺C i ⫽0.

具 H i 典 ⫽ 31 共 H i/x ⫹H i/y ⫹H i/z 兲 .

Since the demagnetizing factors satisfy the conditions: N x ⫹N y ⫹N z ⫽1 and N x ⫽N y then, effective data on particle shapes are reduced to the only parameter N z . The internal field 具 H i 典 , then, becomes

具 H i典 ⫽

冋

册

2 H 1 ⫹ . ⫹ 共 i ⫺ 兲共 1⫺N z 兲 /2 ⫹ 共 i ⫺ 兲 N z 3 共3兲

In the meaning of the effective medium theory applied to the isotropic case, we choose to define5,6 the effective shape factor N by taking for 具 H i 典 the same formal expression as that of the H i components

共1兲

The magnetic susceptibility of the mixture depends on the intrinsic susceptibility i of the magnetic substance as well as on the magnetic volume fraction C, and then on the so-called effective shape factor N for the global representation of the microscopic demagnetizing effects. The next part of our study details how the factor N can be connected to the shapes of particles and to their distributions in space.

具 H i典 ⫽

H . 1⫹ 共 i ⫺ / 兲 N

共4兲

The equality between relations 共3兲 and 共4兲, then, allows us to connect N, first to the real parameter of shape N z of the magnetic particles, and second to the volume fraction C. The effective shape factor N is then given by

II. THEORETICAL DEVELOPMENT

In order to simply calculate the effective factor N, we assume that the particles of concern can be replaced by ellipsoids whose the associated triplet of demagnetizing constants (N x , N y , N z ) is fixed by the ratios of the respective lengths of their semi-axes. One can, then, calculate the diagonal tensor4 of the internal field, H i , for such ellipsoid particles of permeability, i , embedded in a homogeneous medium of permeability, 共Fig. 1兲.

N⫽

2⫹3 ␦ N z 共 1⫺N z 兲 , 6⫹ ␦ ⫹3 ␦ N z

共5兲

where ␦ ⫽ i /(1⫹ ) is a so-called factor of contrast, which itself depends on the volume fraction C. The values of N are calculated by solving Eqs. 共1兲 and 共5兲 together. Figure 2 shows that the effective shape factor N depends both on the magnetic load C and on the real shape factor N z of particles. For separated spherical particles N is equal to 1/3 over the whole volume fraction range. On the other hand, in all other cases, i.e., needle- or flake-type par-

a兲

Electronic mail: [email protected]

0021-8979/2001/90(7)/3462/4/$18.00

共2兲

3462

© 2001 American Institute of Physics

Downloaded 19 Oct 2001 to 193.54.253.44. Redistribution subject to AIP license or copyright, see http://ojps.aip.org/japo/japcr.jsp

J. Appl. Phys., Vol. 90, No. 7, 1 October 2001

A. Chevalier and M. Le Floc’h

3463

FIG. 3. Experimental variations of the real part ⬘ of susceptibility of Ni0.7Zn0.3Fe2O4 magnetic composites. FIG. 1. Components of the internal field H i .

ticles, N is smaller than 1/3 so that the shape anisotropy of particles, even for an isotropic mixture, always has the direct consequence to systematically lower the effective shape factor of the mixture. We will now show the ability of the above analytical model 关Eqs. 共1兲 and 共5兲兴 to predict the dynamic properties of soft magnetic powders. In the example chosen, the model is applied to the extraction, from experimental data, of the intrinsic susceptibility i of the magnetic matter. III. EXPERIMENTAL RESULTS

The fine magnetic powders used in our study were synthesized in our laboratory by a wet method7 in order to be sure of the very high chemical purity of the resulting fine powders. Observations by electron microscopy showed that most of the particles were regular and spherical with diameters close to 0.1 m. However, in agreement with the earlier theory, one should keep in mind that clusters can strongly deviate the magnetic properties of the macroscopic body. Composites materials were made by mixing nonmagnetic 共epoxy resin兲 with soft magnetic (Ni0.7Zn0.3Fe2O4 ferrite兲 powders. Then, they were shaped and pressed at room temperature in ring-shaped matrices to avoid the sample de-

FIG. 2. Effective shape factor N as a function of the magnetic load C and of the particle shape factor (N z ). Theoretical values are obtained by solving the couple of Eqs. 共1兲 and 共5兲 for i ⫽20.

magnetizing fields. The magnetic volume fraction ranged within a few percent to about 60%. Thermal densifications were not used in this study. The initial dynamic susceptibility of the composite material 关 ( )⫽ ⬘ ( )⫺ j ⬙ ( ) 兴 was investigated at room temperature in the frequency range 50 MHz–20 GHz by using a Hewlett-Packard APC7 coaxial-line technique and network analyzers. The results are shown in Figs. 3 共real parts兲 and 4 共imaginary parts兲 for different magnetic fractions in the earlier mentioned range. The reduction of the magnetic load lowers the magnitude of the susceptibility. This behavior is general and usually expected. However, as the magnetic resonance frequency 共MRF兲 is spotted by the maximum of the imaginary part of susceptibility, its behavior is clearly different: first, it remains unchanged, then increases continuously below a certain threshold C p close to 30%. We consider this resonance frequency shift as being a direct consequence of the increase of the microscopic demagnetizing fields in the mixture in connection with the modifications of dipolar-type interactions on the one hand, and of the particle arrangements on the other hand. This is quite consistent with other studies which have also clearly highlighted the basic role of the demagnetizing effects8 on the dynamic properties of the magnetic susceptibility in composite materials. As the volume fraction decreases, the local demagnetizing fields add to the total anisotropy field and consequently increase the resonance frequency. In the next

FIG. 4. Experimental variations of the imaginary part ⬙ of susceptibility of Ni0.7Zn0.3Fe2O4 magnetic composites. Full circles 共䊉兲 spot the resonance frequency shift.

Downloaded 19 Oct 2001 to 193.54.253.44. Redistribution subject to AIP license or copyright, see http://ojps.aip.org/japo/japcr.jsp

3464

J. Appl. Phys., Vol. 90, No. 7, 1 October 2001

FIG. 5. Real part of the dynamic intrinsic susceptibility i⬘ obtained with the inversion of experimental data of Fig. 3.

section we will demonstrate that the model proposed in this study takes properly this internal effect into account. IV. COMPARISONS WITH THE MODEL

To process experimental data in order to extract the intrinsic susceptibility of the magnetic matter, we use Eq. 共1兲 in which i is taken as the unknown variable, whereas C and come from measurements. N is then adjusted under the obvious condition that it must remain less than or equal to 1/3. This leads to the noteworthy transformation of Figs. 3 and 4 into the reduced curves of Figs. 5 and 6. One should, indeed, note that, over the whole frequency range and for the different magnetic fractions, there is a unique solution for N; in consequence, the model we use 关see Eq. 共1兲兴 can describe both the decreasing magnitude of the susceptibility and the shift in the MRF observable in composites magnetic materials. Figure 7 shows the experimental values of the earlier solution for N. They correspond to the expected intrinsic susceptibility and are absolutely consistent with the theoretical curves predicted in Fig. 2. They are not only less than 1/3, but they also depend on the volume fraction. V. DISCUSSION

We showed in the previous section that the effective shape factor N depends on both the real particle shape (N z ) and the magnetic fraction C 关Eq. 共5兲兴. Thus, theoretically in the case of spherical particles, the effective shape factor N must be equal to 1/3 and not depend on the magnetic fraction 共see Fig. 2兲. However, experimental values are systematically below 1/3 and magnetic fraction-dependent even in the case of spherical magnetic particles 共Fig. 7兲. This discrepancy, in fact, results from the unavoidable aggregations of

FIG. 6. Imaginary part of the dynamic intrinsic susceptibility i⬙ , obtained with the inversion of experimental data of Fig. 4.

A. Chevalier and M. Le Floc’h

FIG. 7. Experimental and theoretical values of the effective shape factor N obtained to superimpose dynamic spectra of Figs. 5 and 6.

particles during the powder mixing processes, particularly when they are of very small sizes. By way of consequence the clusters are perceived as new particles distorted and bigger than the others. It is then obvious that the shape distribution of such aggregates cannot be evaluated by direct 共microscopy兲 observations, especially because they are sensitive to the changes in the magnetic load. This is, in fact, quite a general problem which largely goes beyond the limits of this study. It is, however, quite possible from simple and practical assumptions to build an intuitive function of distribution of the cluster shapes. First, any aggregation of individual ellipsoidal particles necessarily results in clusters of ellipsoidal shapes with a demagnetizing factor N z 共see Fig. 8兲. Second, the probability P(N z ) to find clusters with a given shape depends on the magnetic fraction as follows: at low concentrations, the particles tend to remain linked in small chainlike aggregates so as they are equivalent to prolate ellipsoids,9 and then the composite becomes equivalent to a mixture of needle-type particles for which N z is by definition less than 1/3. On the contrary, at high concentrations, the clusters grow in any direction and progressively tend to become spherical: by definition, N z is here equal to 1/3. In our study we considered that the probability to develop flake-like aggregates for which N z is by definition higher than 1/3 was unrealistic.

FIG. 8. Identification of aggregates with ellipsoid.

Downloaded 19 Oct 2001 to 193.54.253.44. Redistribution subject to AIP license or copyright, see http://ojps.aip.org/japo/japcr.jsp

J. Appl. Phys., Vol. 90, No. 7, 1 October 2001

A. Chevalier and M. Le Floc’h

3465

When the particle concentration in a given mixture is increasing, aggregates are rapidly formed; their shapes are, then, continuously changing from chains to spheres up to the concentration unity where the medium becomes isotropic. A further work would be in deriving a mathematical function of the distribution P(N z ) to have finally a completely predicting model. This is an interesting challenge because it is known that the dynamic properties of magnetic powder materials are largely influenced by such a term.

VI. CONCLUSION

FIG. 9. Statistical distribution P(N z ) of aggregates shape (N z ) with the volume fraction C.

The earlier assumptions are sufficient to design a convincing profile of the distribution law P(N z ). Indeed, as the magnetic concentration increases, the function P(N z ) must have a maximum whose position is shifted towards the high values of N z up to 1/3 共strictly speaking兲 when the magnetic fraction reaches unity. Simultaneously, the profile of P(N z ) must become narrower and narrower. Figure 9, finally, shows the histogram of P(N z ) which was used to realize the very satisfactory fit of Fig. 7. For an exact computation of the effective shape factor N, Eq. 共3兲 can be now easily expressed as a continuous sum acting on N z as follows:

具 H i典 ⫽

冕 冋 1

0

⫹

2 ⫹ 共 i ⫺ 兲共 1⫺N z 兲 /2

册

H 1 P 共 N z 兲 dN z . ⫹共 i⫺ 兲N z 3

共6兲

An extension of the effective medium theory was proposed to predict the dynamic behaviors of isotropic composite materials. This model is capable of describing experimental results, namely the variation of magnitude of permeability, together with the shift of the resonance frequency. While taking into account the formation of particle aggregates, we derived the intrinsic permeability of magnetic matter independently of the magnetic fraction of the mixture. An immediate and interesting extension of this work would be the determination of an analytical function of the magnetic fraction of the mixture to take the grain structure contribution into account.

1

J. L. Greffe and Grosse, Dielectric Properties of Heterogeneous Materials, P.I.E.R. 6 共Elsevier, New York, 1992兲. 2 D. A. G. Bruggeman, Ann Phys. 共Leipzig兲 24 共1935兲. 3 M. Le Floc’h, J. L. Mattei, P. Laurent, O. Minot, and A. M. Konn, J. Magn. Magn. Mater. 140 共1995兲. 4 J. A. Stratton, Electromagnetic Theory 共McGraw-Hill, New York, 1941兲. 5 M. Le Floc’h, A. Chevalier, and J. L. Mattei, J. Phys. IV 8, 2 共1998兲. 6 A. Chevalier, Ph.D. thesis, Universite´ de Bretagne Occidentale, 1998. 7 T. Takada and M. Kiyama, Proc. Of Intern. Conf., Japan 1970, p. 69. 8 C. Kittel, Phys. Rev. 73, 155 共1948兲. 9 C. G. Granqvist and O. Hunderi, Phys. Rev. B 18, 1554 共1978兲.

Downloaded 19 Oct 2001 to 193.54.253.44. Redistribution subject to AIP license or copyright, see http://ojps.aip.org/japo/japcr.jsp